Comparative assessment of green and chemically synthesized glutathione capped silver nanoparticles for antioxidant, mosquito larvicidal and eco-toxicological activities

A comparative assessment of AgNPs synthesized through three different routes viz. clove bud extract mediated AgNPs, sodium borohydride AgNPs and Glutathione (GSH) capped AgNPs for antioxidant and mosquito larvicidal activities was the major focus of the present study. The nanoparticles were characterized using UV–VIS spectrophotometry, dynamic light scattering (DLS), X-ray diffraction (XRD), field emission-scanning electron microscopy (FE-SEM), transmission electron microscopy (TEM) and Fourier Transform Infrared Spectroscopy (FTIR) analysis. Characterization studies revealed the synthesis of stable, crystalline AgNPs measuring 28 nm, 7 nm and 36 nm for green, chemical and GSH-capped AgNPs respectively. FTIR analysis exhibited the surface functional moieties that were responsible for reduction, capping and stabilizing AgNPs. Antioxidant activity was found to be 74.11%, 46.62% and 58.78% for clove, borohydride and GSH-capped AgNPs respectively. Mosquito larvicidal bioactivity of AgNPs against Aedes aegypti IIIrd instar larvae depicted clove AgNPs being most effective (LC50—4.9 ppm, LC90—30.2 ppm) followed by GSH-capped (LC50—20.13 ppm, LC90—46.63 ppm) and borohydride AgNPs (LC50—13.43 ppm, LC90—160.19 ppm) after 24 h. Toxicity screening against aquatic model Daphnia magna revealed Clove mediated and GSH-capped AgNPs to be safer as compared to the borohydride AgNPs. It may be envisaged that green and capped AgNPs may be further explored for diverse biomedical and therapeutic applications.


Results and discussion
Synthesis and characterization of AgNPs. This study was aimed for the development of stable, feasible and eco-friendly AgNPs, with good bioactivity. This was done in two ways-preparing AgNPs using clove, as a green approach, using plant material and GSH capping for surface modification of chemically synthesized AgNPs for making them effective, safe and stable. Synthesis of clove AgNPs was visualized through a distinct change in colour of AgNO 3 solution from colourless to dark brown with the addition of aqueous clove extract. Eugenol (4-allyl-2-methoxyphenol), which is the main compound found in clove extract, is responsible for the reduction of silver nitrate and formation of clove AgNPs. A proton is released from OH group of eugenol, creating negative charge on it. The release of two electrons from resonating structure of anionic form of eugenol in this process are responsible for the reduction of 2 Ag+ ions to 2 Ag0. Eugenol, also acts as a capping agent and stabilizes the formed AgNPs 16 .
For the nanoparticles prepared using sodium borohydride, colour change from transparent to yellow indicated the formation of AgNPs. Herein, sodium borohydride facilitated the reduction of AgNO 3 solution. While for the synthesis of GSH-capped AgNPs, dark yellow colour after addition of capping agent-GSH, indicated the www.nature.com/scientificreports/ completion of capping process. The surface of AgNPs is positively charged, while the acetyl (-COO) and thiol (-SH) group of GSH are negatively charged. So, the stabilization of [Ag(GSH)] is due to formation of van der walls forces between these opposite charges. Ionic surface stabilizing agent adsorbs on the surface of AgNPs and generates uniform charge on particle surface, this results in the formation of uniform and stable size particles, with no aggregation 17 .
UV-Vis spectrophotometric analysis. Synthesis of AgNPs was monitored using UV-Vis Spectral analysis. Spectral peaks of synthesized AgNPs are shown in Fig. 1. Spectral peak of green synthesized AgNPs using clove extract was recorded at 439.2, while borohydride AgNPs showed a distinct peak at 388 nm. The spectral peak of GSH-capped AgNPs was observed at 400.8 nm. Our spectral study for GSH-capped is in line with the earlier reported work 18 . AgNPs exhibit a characteristic surface plasmon resonance (SPR) band at or around 400 nm. Spectral peaks of all three types of AgNPs in our study were near or around 400 nm, confirming the formation of AgNPs.
DLS and zeta potential analysis. DLS-size distribution and zeta potential studies were done to examine the hydrodynamic size, type of charge and stability of synthesized AgNPs, as shown in Fig. 2 www.nature.com/scientificreports/ Stability of all three types of synthesized AgNPs was examined through zeta potential. For AgNPs to be stable the value of zeta potential should be around ± 30 mV. The values obtained for clove AgNPs, borohydride AgNPs and GSH-capped AgNPs were as follows: − 28.5 mV, − 18.6 mV and − 23.5 mV. All the values were negatively charged and sharp, showing the surface of AgNPs to be negatively charged and dispersed in medium. The negative value also shows high electrostatic repulsion among the nanoparticles, thus preventing agglomeration and making them highly stable. All three types of AgNPs exhibited high zeta potential, however, clove AgNPs were found to be most stable, with highest zeta potential value. Moreover, zeta potential value of GSH-capped AgNPs was higher compared to borohydride AgNPs clearly indicating the importance of capping in adding stability to AgNPs. Figure 3 shows the XRD data, which confirms the crystalline nature of the synthesized AgNPs. XRD data shows the diffraction peaks at 38.09°, 44.59° and 64° corresponding to (111), (200) and (220) planes of face-centred cubic crystal structure of metallic silver. This was found with all three types of synthesized AgNPs.

FE-SEM and EDX analysis.
FE-SEM clearly shows the shape and morphology of synthesized AgNPs, as shown in Fig. 4. The clove AgNPs were roughly spherical and evenly distributed. Few rod-shaped individual particles were also seen in clove AgNPs, but majority of particles were spherical in shape (Fig. 4a). Borohydride AgNPs were roughly spherical and aggregated (Fig. 4b). While chemically capped AgNPs were spherical, evenly distributed with small size (Fig. 4c). EDX analysis revealed presence of silver in all three types of synthesized AgNPs, Ag element shows a characteristic signal peak at 3 keV, due to surface plasmon resonance, which indicates the presence of silver in the system 19 . Silver (Ag) representative signal peak was observed near 3 keV (Lα) in all the AgNPs under study. Figure 4 also shows the quantitative element details of different AgNPs. The presence of elements apart from main Ag element like Na, Ca and Mg in clove AgNPs could be accounted to secondary metabolites present in clove extract, which are very crucial for nanobiosynthesis of AgNPs. Similar results have been reported for AgNPs synthesized using Pedalium murex leaf, which also had presence of elements like O, C, K, Ca, Cl and Na. This may be accounted for metabolites and functional moieties present in Pedalium murex leaf extract used for preparing AgNPs 20 . Apart from this presence of C and O element in borohydride and GSHcapped AgNPs could be accounted to the grid used in FE-SEM study. TEM analysis. TEM was done to study in details, the size and distribution of particles. TEM micrographs and the corresponding particle size distribution histogram of AgNPs obtained by TEM images are presented in Fig. 5. TEM micrographs of clove AgNPs clearly showed spherical shape AgNPs, with size around 28 nm www.nature.com/scientificreports/ (Fig. 5a). Similar size range was also found in AgNPs prepared using extracts of Tectona grandis seeds extract 21 .
Possible reasons for the similar size range could be accounted to similar concentrations of extract used in preparation of AgNPs and presence of various phytopotentials moieties in the prepared AgNPs, due to the use of green compounds. Chemically synthesized AgNPs were spherical measuring 7 nm (Fig. 5b) whereas, GSH-capped AgNPs revealed spherical particles with slight aggregation measuring around 36 nm (Fig. 5c). The comparison between the sizes of borohydride AgNPs and GSH-capped AgNPs, clearly shows the role of GSH capping in enhancing the particle size. Results of particle size obtained from DLS studies were larger compared to their size revealed through TEM results. Our results found correlation with study on AgNPs prepared using Pedalium murex leaf extract, in which DLS size was 23 nm larger than the TEM size of prepared AgNPs 20 . In another case, of Zirconia nanoparticles, the difference in size of nanoparticles given by DLS was higher by a factor of two to three compared to size analyzed for same nanoparticles by TEM technique 22 . Larger size found in DLS studies compared to TEM could www.nature.com/scientificreports/ be explained with the fact that TEM analysis delineates actual particle size while DLS provides hydrodynamic size representing a sum of particles, hydration sphere and surfactant agent shell coverage hence, relatively larger size of nanoparticles. Moreover, DLS is measured in solution form, with a solvent layer, and thus has tendency to aggregate, while for TEM analysis samples are dried, and thus provides actual size.
FTIR analysis. Figure 6 presents FTIR analysis which provides information about different functional groups and this spectral study is important for deciphering interactions resulting in reduction, adsorption and forma-  www.nature.com/scientificreports/ tion of AgNPs. Analysis was done in the spectral window of 500 to 4000 cm −1 . FTIR spectra of clove AgNPs was done to elucidate knowledge about the chemical changes occurring in functional moieties of phytopotentials of clove bud extract, upon being adsorbed on the AgNPs surface and their participation in bioreduction of silver metal. A small peak was recorded at nearly 3700 cm −1 corresponding to O-H stretching of free hydroxyl groups of alcohol and phenols. Apart from this, a broad peak was also observed between 3550 and 3200 cm −1 corresponding to intermolecular bonded O-H group of residual eugenol 16 . A small peak was observed at 2600 cm −1 corresponding to S-H thiol group. Also, a tiny stretch found at 2150 cm −1 which may be accounted for ketene group. From literature, it is evident that band at 1650 cm −1 corresponds to C=O is not found in clove extract, while appearance of this band in clove AgNPs spectra is proof of involvement of eugenol in bioreduction process and formation of AgNPs 23 . Thus, it indicates the formation of clove AgNPs capped with different bio moieties 24 .
The IR spectrum showed a peak at 1098 cm −1 corresponding to C-O (carboxylic acid derivative) stretching, formed in eugenol after bioreduction of silver. A very sharp and intense peak was obtained at 650 cm −1 corresponding to R-CH alkane functional group, which are abundantly found in clove extract. These observations confirmed the presence of eugenol and other functional moieties (mainly water-soluble flavonoids), which acts as reducing and stabilizing agent in the synthesis of clove AgNPs. In borohydride AgNPs, several peaks with high intensity were obtained because of interaction of chemical NaBH 4 with AgNO 3 . Stretches of O-H were also recorded between 3700 and 3500 cm −1 corresponding to free hydroxyl and H-bonded alcohol and phenol groups. A broad stretch was recorded between 3500 and 3300 cm −1 corresponding to N-H aliphatic primary amine. Peaks recorded at 2800 cm −1 corresponded to aliphatic C-H bending vibrations while a small, weak band was observed at 2550 cm −1 upper side, corresponding to S-H thiol group. A Significant peak was detected at 2260 cm −1 , which could be attributed to C≡N nitrile stretching whereas, a small vibration was observed at 2100 cm −1 , corresponding to alkyne (C≡C) however, a sharp and strong peak was noticed at 1620 cm −1 , which could be assigned to C=C α, β unsaturated ketone. A very sharp and intense peak was also obtained at 1423 cm −1 which could be accounted to be generated by the borohydride anion of NaBH 4 , that remained partly bound to the AgNPs and corresponded to C-H bending. Moreover, stretch at 800 cm −1 corresponds to aliphatic C-H bending vibrations of alkanes.
The interactions of AgNPs with GSH were confirmed by the absence of N-H and S-H stretching bands, which are otherwise present in pure GSH and found at 3350 cm −1 and 2600 cm −1 respectively 11 . The absence of spectral peaks of S-H and N-H, suggest that glutathione is modified onto the surface of AgNPs by the thiol and amine groups from the cysteine moiety of Glutathione. These findings are supported by a previous study where a small spectral stretch resembled our FTIR analysis 17 however, as different conditions such as heating and longer stirring hours were used by them, there were some deviations in the present spectra. Additionally in the study, a broad peak was observed between 3550 and 3200 cm −1 corresponding to O-H stretching of intermolecular bonded alcohol. Also, a small stretch at 2140 cm −1 was found, which can be assigned to alkyne (C≡C). Apart from this, a very sharp and intense peak was obtained at 1650 cm −1 for C=O stretch representing α, β unsaturated aldehydes and ketones. One more distinct peak was also obtained at 1250 cm −1 which represents C-N functional group of aliphatic amines. Vibration of C-H bond due to alkanes and aromatic generated two sharp peaks of same intensity at 870 cm −1 and 750 cm −1 . A small band was also pointed at 890 cm −1 representing C-H group trisubstituted bonding. The broad peaks from 639 to 500 cm −1 are related to Ag-NPs bonding with sulphur from thiol groups of GSH molecules. Antioxidant activity. Radical scavenging activity is a measure of scavenging of free radicals which are generated in the form of reactive oxygen species (ROS). DPPH is a free radical capable of accepting an electron or hydrogen radical to become a stable molecule and it has an absorption maximum at 517 nm. Radical Scavenging Activity (RSA) of different synthesized AgNPs viz., clove (green), NaBH 4 (uncapped) and GSH (capped) were evaluated. The radical scavenging activity was found to be concentration dependent. Figure 7 depicts the RSA values of the synthesized AgNPs. Ascorbic acid was used as a standard (gave RSA value of 97.17% at 100 ppm conc.) Radical scavenging efficacy of clove AgNPs was found to be the highest among all the samples-58.42% to 74.11%. These results correlate with the other findings done on antioxidant activity of Leptadenia reticulata and Ananas comosus 25,26 . The percent RSA of chemically synthesized AgNPs i.e., borohydride AgNPs ranged from 33.34 to 46.62%, which was lower than percent RSA value of AgNPs synthesized from www.nature.com/scientificreports/ clove, moreover the percent RSA values of GSH-capped AgNPs was found to be in the range of 33.89-58.78%, which were lower than the percent RSA values of clove AgNPs but higher than borohydride AgNPs. The decreasing order of radical scavenging activity was as follows: clove AgNPs > GSH-capped AgNPs > Borohydride AgNPs. Chemically synthesized NPs were found to have least percent RSA value (46.62%) among all samples, the reason for this may be accounted to the free ends of chemically synthesized AgNPs which generates free radicals. GSHcapped AgNPs were found to have increased antioxidant efficacy than borohydride AgNPs, which may be due to the capping which probably reduced the free ends of AgNPs resulting in less generation of free radicals. Free radical generation is associated with nanotoxicity and enhancing the antioxidant activity seems to be a promising solution to manipulate the surface properties of nanoparticles imparting stability through thiol rich moieties either chemically or green route.

Mosquito larvicidal bioactivity.
Mosquito larvicidal potential of synthesized AgNPs was determined against III instar larvae of Dengue vector Aedes aegypti under laboratory conditions. Control group showed mortality only at 72 h. Mean percent mortality at different concentrations at 24 h, 48 h and 72 h of green, chemically synthesized as well as capped AgNPs was found out. Various mortality patterns were observed at different concentrations and are shown in Fig. 8. Clove mediated AgNPs were found to be very effective and exhibited high mean percent mortality even at 24 h. At the lowest concentration, clove AgNPs showed mean percent mortality of 21% which reached up to 96% with the highest concentration and at 72 h this range increased from 45 to 98%. Borohydride AgNPs showed lower mean percent mortality as compared to that of clove AgNPs. Their mortality range was found to be between 11 and 73% at 24 h and at 72 h it extended from 23 to 98%. For GSH-capped AgNPs, after 24 h, the mortality was in the range of 1-68%, and then at 72 h it reached from 21 to 88%. Similar results are also reported by various other researchers on dengue vector 27,28 .  www.nature.com/scientificreports/  24 h. Green nanoparticles were found more effective owing to the phytopotentials involved. On the other hand, nanoparticles are known to trigger free radical activity on the surface of the particles whereas, capping enhances their scavenging activity as free sites becomes enclosed and reduces the nanotoxicity making them suitable for benign application in various fields. Hitherto, this is the first study where three different types of AgNPs were synthesised using different routes and compared for their different activities and a way is figured out to make the AgNPs much stable and potent for larvicidal applications.
Acute toxicity of AgNPs to D. magna. Toxicity assessment of AgNPs is important to understand the risk associated with AgNPs to the environment, hence, 48 h toxicity was evaluated for all the three AgNPs and compared with controls. Percent survivability of D. magna neonates treated with various AgNPs, at the highest test concentration depicted 80% and 60% survivability with clove and GSH-capped AgNPs respectively, while, exposure with borohydride AgNPs resulted in 100% mortality. Figure 9 shows the range of percent survivability for all the three AgNPs i.e., clove AgNPs (90-80%), borohydride AgNPs (60-0%) and GSH-capped AgNPs (90-60%) at various test concentrations. Higher survivability percentage with clove AgNPs could be due to the phytopotentials of botanical extract, that posed least threat to the eco-toxicity model organism D. magna. On the other hand, higher mortalities on exposure with borohydride AgNPs could be assigned to the chemicals employed during their synthesis, which might have interacted with the cellular and sub-cellular components of D. magna and generated oxidative stress, resulting in lesser or no survivability of the test organism. Surprisingly, GSH-capped AgNPs demonstrated higher survivability which was comparable with the green clove AgNPs. It may be deduced from these findings that this moderate to low toxicity could be due to capping of the free ends of these AgNPs, culminating into stabilized AgNPs with least toxicity and safer action as hypothesized in this study. Further, this finds support with the antioxidant activity of GSH-capped AgNPs that was enhanced as compared to the chemically synthesized borohydride AgNPs. The swimming behaviour of D. magna neonates was also observed in all three AgNPs treatment groups and compared with that of controls. It was noticed that control and clove AgNPs treated D. magna neonates showed normal swimming behaviour both after 24 h and 48 h, while borohydride AgNPs treatment slowed down their movement after 24 h and further after 48 h con-  www.nature.com/scientificreports/ centrating mainly at bottom. GSH-capped AgNPs treated neonates showed somewhat transitional swimming behaviour between other two treatment groups.

Morphological alterations in D. magna observed by phase-contrast microscopy.
Morphological alterations of D. magna were observed and recorded after 48 h acute toxicity assay (Fig. 10) and compared with that of the control. Control specimen showed healthy neonate with no morphological alterations. D. magna following treatment with the clove AgNPs, not much deviation from the controls could be noticed. On the contrary, borohydride AgNPs treated neonates demonstrated various morphological alterations such as overall carapace and lining of internal structures became lighter giving the hyaline appearance as compared to other treatment groups. AgNPs accumulation at the hindgut region, internal fluid leakage from ephippium due to carapace rupturing, disrupted gut region and mouth parts were other major alterations apparently noticeable. Since, D. magna is a bottom level filter feeding organism and occupies lower level in food chain and trophic level, any form of nanoparticles accumulation in this organism, may results in transferring nanoparticles and its toxicity to higher level organisms in food chain too 29,30 . Interestingly, GSH-capping to these AgNPs greatly reduced their toxicity as most of the structures were intact and slight pigmentation was found both in foregut and midgut. Major morphological alterations in borohydride AgNPs treated neonates, clearly depicts its higher toxicity as compared to other two AgNPs. The toxicity assay results clearly indicate the non-toxic nature of green AgNPs and also highlights the effectiveness of capping in imparting stability and safety to chemical AgNPs.

Materials and methods
Green synthesis of AgNPs. The synthesis of AgNPs was done using a previously reported method, with some modifications 13 . Clove buds were purchased from the local dealer. Various percentages of aqueous extracts (1%, 2%, 3%, 4%, 5% and 10%) were prepared using microwave assisted protocol and filtered. The extract was rich in thiol moieties due to eugenol (4-allyl-2-methoxyphenol) thus acting as a reducing, stabilizing and capping agent and was used for the green synthesis of AgNPs. 10 ml of each of these was mixed with 90 ml of 1 mM silver nitrate (AgNO 3 ) solution respectively. The change in colour of solution from colourless to amber and finally to a dark brown colloidal solution indicated the formation of AgNPs. Spectra were taken to monitor the synthesis of extract mediated AgNPs. No distinct absorption peaks could be for 1%, 2%, 3% and 4% however, absorbance and surface plasmon resonance bands were found similar for 5% and 10%, thus 5% was selected for this study taking cost effectiveness into consideration.
Chemical synthesis of AgNPs. Chemically, AgNPs were prepared using AgNO 3 as precursor and sodium borohydride (NaBH 4 ) as a reducing agent. Briefly, 100 ml of 0.25 mM AgNO 3 was prepared with continuous stirring. Freshly prepared 0.1 M NaBH 4 (150 ml) was taken into the conical flask and kept on the ice bath for half an hour. To this solution drop by drop AgNO 3 was added at the rate of 1 drop/s. Colour change was noticeable (pale brown), which indicated the formation of AgNPs 31 .

Synthesis of glutathione (GSH)-capped AgNPs. Surface modification of borohydride AgNPs by GSH
was done with some modifications in protocol of Chandraker et al. 10 . Briefly, 100 ml AgNO 3 (0.23 nM) was prepared, to which freshly prepared 10 ml NaBH 4 (0.1 M) was added, with continuous stirring for 30 min. After that, ethanolic GSH was prepared by mixing 0.05 g of GSH in 10 ml ethanol and it was added to the above solution. pH was adjusted to 11.67, using dilute NaOH. The prepared solution was kept in dark with constant stirring for 20 h. Colour change from pale yellow to dark yellow indicated the AgNPs surface modification by GSH capping. www.nature.com/scientificreports/ (Department of Zoology, DEI, Agra) for monitoring the reduction of pure silver ions at different intervals. The spectra were measured in wavelength range between 300 and 700 nm. Hydrodynamic size, distribution and stability analysis of AgNPs were evaluated by Zetasizer instrument (Malvern, UK) (SAIF, AIIMS, New Delhi) by measuring DLS and Zeta potential. PdI (Polydispersity Index) was also measured for determining the width of particle size distribution. For DLS analysis samples were diluted with milli Q water (1:4) to avoid multiple scattering effects. Measurements were performed in triplicates. The temperature equilibration time was 1 min at 25 °C and data processing was set to high multi-modal resolution. XRD (X-Ray Diffractometer) measurements were done to study the crystal structure. XRD was performed using a Bruker AXS D8 advance diffractometer, Germany (Central facility Department of Chemistry, DEI, Agra) having Cu Kα 1 (λ = 1.54060 Å) radiation at 40 kV and 30 mA. Detailed morphology and size, shape analysis was done using FE-SEM (Field Emission Scanning Electron Microscope) JEOL JSM-7610FPlus, Japan (Central facility Department of Chemistry, DEI, Agra). Samples were analyzed after drying and platinum coating at 20 kV. Elemental analysis was done using EDXS (Energy Dispersive X-ray Spectroscopy) equipped with FE-SEM. Further TEM (Transmission Electron Microscope) analysis was done to analyze exact shape, size and morphology of different AgNPs. This was done using Thermo Scientific Talos 33 . Various test concentrations of AgNPs were prepared from stock. A preliminary experiment was set up to decide effective concentration from broad concentration ranges. Following concentrations were selected for the AgNPs toxicity testing-0.001 ppm, 0.005 ppm. 0.01 ppm, 0.05 ppm, 0.1 ppm. Less than 24 h old neonates form third brood progeny were selected. 10 neonates were placed in 250 ml beakers containing 100 ml test concentrations. quadruplicate of each test concentration and control was put. Test were done in optimum conditions temperature (20 ± 2 °C) and 16:8 h light-dark cycles respectively and dissolved oxygen concentration was higher than 3 mg L −1 in each test set. No food was given during test period, as organic matters affect intake of NPs in the test organism, thus affecting and wrongly modifying the overall result. Percent survivability was recorded after 24 h and 48 h and swimming behaviours were also observed. Test organism was considered dead, when it showed no observed movement in post-abdomen or appendages within 15 s of gentle agitation of test container 34 . The toxicity tests were considered valid, if mortality in control was less than 10%. Morphological alterations in test organism after 48 h toxicity assay were recorded using OPTIKA phase contrast microscope (IM-3), Italy, having slider with phase Rings (4×/10×, 20×/40×).

Statistical analysis.
Value of mean percent mortality, radical scavenging activity and toxicity assay are represented in mean ± standard deviation. Larvicidal susceptibility is expressed in terms of LC 50 and LC 90 using probit analysis 35 . Acute toxicity assay is expressed in terms of survival percentage. Control mortality was corrected using the Abbott's formula 36 . ORIGIN 9.0 software was used in generating graphs.

Conclusions
This is first ever comparative study of green and chemically synthesized GSH capped AgNPs for evaluating their bioactivities and eco-toxicity screening. Concludingly, the present study clearly elucidates that among the three types of AgNPs, clove AgNPs had highest antioxidant and mosquito larvicidal bioactivity followed by GSHcapped AgNPs and borohydride AgNPs. This study also highlights that GSH capping greatly reduced toxicity through stabilization of the free ends of chemically synthesized AgNPs validating our hypothesis of safer synthesis of AgNPs. It may be envisaged that utilizing botanicals and also capping of chemical nanoparticles are excellent ways for the synthesis of small sized and effective nanoparticles, and these can be further explored for diverse biomedical and therapeutic applications and bioactivities.

Data availability
All data generated or analysed during study are included in this published article however, may be made available on further reasonable request from corresponding author.